Quasi-1D chains of dinickel lantern complexes and their magnetic properties.
Nimthong-Roldán, Arunpatcha; Guillet, Jesse L.; McNeely, James; Ozumerzifon, Tarik J.; Shores, Matthew P.; Golen, James A.; Rheingold, Arnold L.; Doerrer, Linda H.; Dalton transactions (Cambridge, England : 2003) 46 (2017) 5546–5557; doi:10.1039/c6dt04535a

data_7042304
_publ_section_title
;
 Quasi-1D chains of dinickel lantern complexes and their magnetic
 properties.
;
_journal_issue                   17
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              5546
_journal_page_last               5557
_journal_paper_doi               10.1039/c6dt04535a
_journal_volume                  46
_journal_year                    2017
_chemical_formula_sum            'C12 H16 N2 Ni2 O4 S4'
_chemical_formula_weight         497.93
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2017-01-30 deposited with the CCDC.
2017-02-17 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 112.87(6)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.670(19)
_cell_length_b                   9.658(14)
_cell_length_c                   16.44(2)
_cell_measurement_reflns_used    2149
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      27.465
_cell_measurement_theta_min      2.679
_cell_volume                     1854(5)
_computing_cell_refinement       'SAINT v8.34A (Bruker, 2013)'
_computing_data_collection       'APEX2 v2013.6-2 (Bruker, 2013)'
_computing_data_reduction        'SAINT v8.34A (Bruker, 2013)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'ShelXT (Sheldrick, 2008)'
_diffrn_ambient_temperature      100(2)
_diffrn_detector                 'Bruker APEX-II CCD'
_diffrn_detector_area_resol_mean 7.9
_diffrn_detector_type            'CCD Area Detector'
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measurement_device       'Kappa Four-Circle Diffractometer'
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\w and \f scans'
_diffrn_radiation_monochromator  'Double Bounce Multilayer Mirrors'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0409
_diffrn_reflns_av_unetI/netI     0.0497
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.990
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            6339
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.990
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.689
_diffrn_reflns_theta_min         1.344
_diffrn_source                   'Micro Focus Rotating Anode'
_diffrn_source_type              'Bruker TXS'
_exptl_absorpt_coefficient_mu    2.500
_exptl_absorpt_correction_T_max  0.2617
_exptl_absorpt_correction_T_min  0.1968
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2014/5 (Bruker,2014/5) was used for absorption correction.
wR2(int) was 0.0901 before and 0.0468 after correction.
The Ratio of minimum to maximum transmission is 0.7520.
The \l/2 correction factor is Not present.
;
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    1.784
_exptl_crystal_description       blade
_exptl_crystal_F_000             1016
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.08
_refine_diff_density_max         1.352
_refine_diff_density_min         -0.832
_refine_diff_density_rms         0.159
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.057
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     182
_refine_ls_number_reflns         2151
_refine_ls_number_restraints     228
_refine_ls_restrained_S_all      1.017
_refine_ls_R_factor_all          0.0706
_refine_ls_R_factor_gt           0.0575
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0589P)^2^+21.5929P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1383
_refine_ls_wR_factor_ref         0.1464
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1812
_reflns_number_total             2151
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c6dt04535a2.cif
_cod_data_source_block           Compound_4
_cod_depositor_comments
'Adding full bibliography for 7042304--7042307.cif.'
_cod_database_code               7042304
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              75622